of 13/13
Nov. 25, 2008 Phase Transformation of Materials Nong-Moon Hwang 4.3 Alloy solidification 4.3.2 Eutectic solidification 4.3.1 Solidification of single-phase alloys
• date post

18-Mar-2022
• Category

## Documents

• view

2

0

Embed Size (px)

### Transcript of Phase Transformation of Materials

Microsoft PowerPoint - 2008-11-25Fig. 4.19 A hypothetical phase diagram. k = XS/XL is constant.
No Diffusion on Solid, Diffusional Mixing in the Liquid
Consider the solidification during cooling under the conditions no diffusion on solid and diffusional mixing in the Liquid. What would be the composition profile at T2 < TS/L < T3? What would be the steady state profile at T3? What would be the composition profile at TE and below?
local equil. at S/L interface
no stirring→ diffusion
Fig. 4.22 Planar front solidification of alloy X0 in Fig. 4.19 assuming no diffusion in solid and no stirring in the liquid.
(a) Composition profile when S/L temperature is between T2 and T3 in Fig. 4.19.
(b) Steady-state at T3. The composition solidifying equals the composition of liquid far ahead of the solid (X0).
(c) Composition profile at TE and below, showing the final transient.
No Diffusion on Solid, Diffusional Mixing in the Liquid
No Diffusion on Solid, Diffusional Mixing in the Liquid
Rate at which solute diffuses down the concentration gradient = Rate at which solute is rejected from the solidifying liquid
( )L L S
∂ = − = −

)] )/(
( )L L SJ DX v X X′= − = − L S L
X XX D v −′ = −
∂ = − = −

What would be Te along the concentration profile ahead of the growth front during steady-state solidification?
Fig. 4.23 The origin of constitutional supercooling ahead of a planar solidification front. (a) Composition profile across the solid/liquid interface during steady-state solidification. The dashed line shows dXL/dx at the S/L interface. (b) The temperature of the liquid ahead of the solidification front follows line TL. The equilibrium liquidus temperature for the liquid adjacent to the interface varies as Te. Constitutional supercooling arises when TL lies under the critical gradient.
Constitutional Supercooling
Cellular and Dendritic Solidification
• Criterion for the planar interface :
TL’/v>(T1-T3)/D : the protrusion melts back. T1-T3 : Equilibrium freezing range of alloy
Large range promotes protrusions.
Development of secondary arms and tertiary arms: <100>
Solute effect : low k enlarges T1-T3 Promotes dendrites.
Cooling rate effect : Fast cooling makes lateral diffusion of the rejected solutes difficult and promotes cell formation of smaller cell spacing.
Fig. 4.24 The breakdown of an initially planar solidification front into cells
Fig. 4.25 Temperature and solute distributions associated with cellular solidification. Note that solute enrichment in the liquid between the cells, and coring in the cells with eutectic in the cell walls.
Fig. 4.26 Cellular microstructures. (a) A decanted interface of a cellularly solidified Pb-Sn alloy (x 120) ( after J.W. Rutter in Liquid Metals and Solidification, American Society for Metals, 1958, p. 243). (b) Longitudinal view of cells in carbon tetrabromide (x 100) ( after K.A. Jackson and J.D. Hunt, Acta Metallurgica 13 (1965) 1212).
Fig. 4.27 Cellular dendrites in carbon tetrabromide. ( After L.R. Morris and W.C. Winegard, Journal of Crystal Growth 6 (1969) 61.)
Fig. 4.28 Columnar dendrites in a transparent organic alloy. ( After K.A. Jackson in Solidification, American Society for Metals, 1971, p. 121.)
4.3.2 Eutectic Solidification (Thermodynamics)
Plot the diagram of Gibbs free energy vs. composition at T3 and T4.
What is the driving force for nucleation of α and β?
What is the driving force for the eutectic reaction (L →α + β) at T4 at Ceut?
Eutectic Solidification (Kinetics)
interlamellar spacing →
If α is nucleated from liquid and starts to grow, what would be the composition at the interface of α/L determined?
→ rough interface → local equilibrium
Nature’s choice?
What would be a role of the curvature at the tip?
→ Gibbs-Thomson Effect
Eutectic Solidification
Critical spacing, * *: ( ) 0Gλ λΔ =
λ = − Δ Δ
What would be the minimum λ?
For an interlamellar spacing, λ, there is a total of (2/ λ) m2 of α/β interface per m3 of eutectic.
( ) ?G λΔ =
2 mG Vγμ
λ → Δ = Δ = ×
L latent heat per unit volume
γ γ = = Δ Δ
0
2 E mT V identical to critical radius H T γλ = − →
Δ Δ
Gibbs-Thomson effect in a ΔG-composition diagram?
Fig. 4.33 (a) Molar free energy diagram at (TE - T0) for the case λ * < λ < ∞ , showing the composition difference available to drive diffusion through the liquid ( X ). (b) Model used to calculate the growth rate.
Corresponding location at phase diagram?
Dr0 TTT Δ+Δ=Δ
total r DG G GΔ = Δ + Δ
2 m r
αγγ λ
α β
c c dl λ Δ = = − =

* *
Δ = Δ − ∝ Δ −
Δ = −
Nature’s choice of lamellar spacing
Fig. 4.34 Eutectic phase diagram showing the relationship between X and X 0 ( exaggerated for clarity )
Fig. 4.29 Al-Cu Al2 lamellar eutectic normal to the growth direction ( x 680). ( Courtesy of J. Strid, University of Lulea, Sweden.)